J Therm Anal Calorim (2012) 110:153–158 DOI 10.1007/s10973-012-2303-9
Dehydration kinetics of Portland cement paste at high temperature Qi Zhang • Guang Ye
CEEC-TAC1 Conference Special Issue Ó The Author(s) 2012. This article is published with open access at Springerlink.com
Abstract Portland cement paste is a multiphase compound mainly consisting of calcium-silicate-hydrate (CSH) gel, calcium hydroxide (CH) crystal, and unhydrated cement core. When cement paste is exposed to high temperature, the dehydration of cement paste leads to not only the decline in strength, but also the increased pore pressure in the paste. In this article, the dehydration kinetic was characterized in term of the combination of kinetics of CSH and CH. The dehydration kinetics data of cement paste at different heating rates was collected by thermogravimetry. The influence of temperature on the reaction rate is analyzed by Arrhenius equation. The Arrhenius parameters of CSH and CH, activation energy, and preexponential factor are determined by isoconversional method. The calculated kinetics parameters were validated by further experimental data finally. Keywords Kinetics Dehydration Cement paste High temperature TG Isoconversional method
Introduction The dehydration of Portland cement paste plays an important role in the concrete structure explosive spalling at fire. Calcium silicate hydrate (CSH) and calcium hydroxide (CH) are the main hydration phases which dominate the properties of Portland cement paste. The temperature range corresponds to the dehydration of CSH is about from 105 to 1,000°C . The temperature range corresponds to the dehydration of CH is about from 400 to Q. Zhang (&) G. Ye Stevinweg 1, 2628 CN Delft, The Netherlands e-mail: [email protected]
550°C. The dehydration of cement paste, together with evaporation of capillary water, has a great influence on the build-up of high pore pressure, which can result to explosive spalling of concrete. The dehydration analysis of cement paste can be facilitated by the use of thermal analysis techniques, including thermogravimetric analysis (TG) and differential scanning calorimetry (DSC). The dehydrations of different cement pastes [1–4] were investigated by TG at given heating rates. The chemical meanings of peaks of TG/DTG curve were qualitatively described [2–4]. The dehydration kinetics of cemetitious materials were usually characterized by the modified Arrhenius equation , where the cemetitious materials were considered as pure substance. However, the dehydration kinetics of Portland cement paste is too complex to be described by a single Arrhenius equation. The dehydration of Portland cement paste is comprised by dehydration of CSH and CH . Moreover, the dehydration of CSH itself is a multi-step reaction [6, 7], in which the Arrhenius parameters (activation energy and pre-exponential factor) vary with dehydration degree. Therefore, it’s difficult to use a single pair of Arrhenius parameters to reveal the chemical mechanism and to predict the dehydration process of cement paste accurately. In this study, the dehydration kinetics of Portland cement paste was characterized as the combination of two parallel kinetics processes, i.e., kinetics of CSH and CH. To confirm that these two reactions dominate the dehydration process, the crystalline composition of cement paste sample was characterized by X-ray diffraction. The dehydration mass losses (TG curves) of cement paste at different heating rates were collected by thermogravimetry for the parameters determination. The TG curves of cement paste were separated into the TG curves of CSH and CH by a graphic method. The dehydration kinetics parameters of
Q. Zhang, G. Ye
CH and CSH were computed, respectively, based on the TG data. The isoconvertional method  was performed to calculate the reaction-degree-dependent activation energy of CSH and CH. This kinetics model and calculated parameters were verified by further experimental data.
Material The experiment were carried out by using an ordinary Portland cement (OPC) CEM I 42.5N. The water/cement ratio was 0.5. The cement paste was cast in small plastic bottles. After curing in closed bottles for 28 days, the hardened paste were removed from the plastic bottles. Before measurement, the cement paste samples were stored in the oven at 105°C for 24 h to remove the free water. The cement paste samples were milled into powders (\50 lm) for thermogrametic analysis.
Method Because the cement paste with age of 28 days was investigated in this study, the possible carbonation in samples is assumed to be negligible. The dehydration process of Portland cement paste is considered as the reactions as following: ðCaOÞa SiO2 ðH2 OÞb ðCaOÞa SiO2 ðH2 OÞbc þ c H2 Ovapor vapor
CaðOHÞ2 CaO þ H2 O
the Friedman model  was used for kinetics of nth-order reaction in this study. f ðaÞ ¼ ð1 aÞn
where n is the reaction order, a is the reaction degree. Arrhenius equation is used to describe the influence of temperature. KðTÞ ¼ A0 exp Ea =RT
where A0, the pre-exponential factor and Ea, the activation energy are referred to as the Arrhenius parameters. Given attention to the reaction order and temperature, the kinetics of dehydration of each phase can generally be expressed as following equation: da ¼ KðTÞf ðaÞ dt
Equation 5 characterizes the dehydration kinetics of CSH and CH. Hence, the global dehydration kinetics of cement paste is considered as the combination of the dehydration kinetics of CSH and CH. The kinetics analysis of CSH and CH is carried out by following four steps:
Crystalline phase identification Portland cement paste is a complex material that might contain some minor hydration products and calcium carbonate (CaCO3). These minor phases can effect the total mass loss of cement paste at high temperature. Therefore, before thermal analysis, the crystalline composition of cement paste must be identified to make sure that the minor phases are negligible in samples, and that dehydration of CSH and CH is the main reaction during heating. The mineral composition of cement paste sample was measured by powder X-ray diffraction (XRD). The X-ray source of ˚ ) was used. The scan step Cu Ka radiation (k = 1.54056 A size was 0.02° in the range 2h from 5° to 70°. Mass loss data collection by thermogravimetric analysis The simultaneous thermogravimetry analyzer was used to measure the TG curves. The purge gas was nitrogen, and the gas velocity was 20 ml/min. The sample was heated from 30 to 1,100°C with different rates: 1, 2, 5, 10 and 30°C/min. Separation of TG curve To study the dehydration kinetics of hydrates separately, the TG curves of cement paste are divided into TG curves due to dehydration of CSH and CH respectively. As Fig. 1 shown, the derivative of mass loss (DTG) has a large peak at around 450°C, which stands for the dehydration of CH. The onset and offset point of dehydration of CH can be determined by the edge of that peak. The mass loss at this segment between the onset and offset is contributed by both the dehydration of CH and CSH. It is assumed that the rate of dehydration of CSH in this segment was the same with the neighbored segments in this study. Therefore, two tangent lines are made through onset and offset, which stand for the mass loss of CSH. The mass loss due to dehydration of CH can be known by calculating the vertical distance of these two trend lines at the midpoint between onset and offset (Fig. 1). By this graphic method, the TG curve of cement paste is separated into TG curves of CSH and CH in Fig. 1. Determination of kinetics parameters by isoconversional method Kinetics parameters vary with extent of conversion at the multi-step kinetics, such as dehydration of CSH. Isoconversional methods employ multiple heating rates in order to obtain data on varying rates at a constant extent of conversion. Thus, isoconversional methods allow multi-step processes to be detected via a variation of Ea with a. The dehydration degree is calculated from TG curves first:
Dehydration kinetics of Portland cement
155 TG of cement paste
TG of CH
TG of CSH
DTG of cement paste
94 Mass loss due to dehydration of CH
Fig. 1 Separation of TG curve of cement paste into TG curves of CSH and CH
wi w0 wfinal w0
where wi is the mass during dehydration, w0 is the initial mass, wfinal is the final mass after dehydration. In this study, isoconversional Friedman method was performed , and the reaction order is assumed to be one: da Ea ln þ lnA þ lnð1 aÞ ¼ dt RT
by plotting ln(da /dt) against 1/T, one directly obtains the slope –Ea/R for a fixed a. And the lnA can be determined by the intercept lnA ? ln(1 - a).
Results and discussion The XRD pattern of dried Portland cement paste is shown in Fig. 2. The crystalline phases are determined. Alite, belite, quartz and brownmillerite are ingredients of unhydrated clinker. Portlandite (CH) is the hydration product. Due to amorphous structure of CSH, the peaks of CSH gel can’t be found in the XRD pattern. Because the samples are isolated with air during curing, the calcite (CaCO3) is not detected in the samples. Therefore, decarbonation of samples during heating is neglected. The mass loss curves of samples under different heating rates were shown in Fig. 3a. A rapid mass loss at around 450°C was observed in each TG curve, that was caused by dehydration of CH. By using the graphic method in Section
Fig. 2 XRD pattern of dried Portland cement paste (oven dried by 105°C)
4000 3500 3000 2500 2000 1500 1000 500 0
‘‘Separation of TG curve’’, the mass loss curves of CH and CSH at different heating rate are determined subsequently in Fig. 3b, c. Both dehydration of CH and CSH were significantly affected by the heating rate, which are shown in Fig. 3b, c. In these figures, it was found that at the same temperature the dehydration degree of the sample with low heating rate is larger than that of the sample with high heating rate. This is because the sample with lower heating rate has more time to dehydrate. It was also found that the temperature range corresponding to the dehydration of CH varies with the heating rate (Fig. 3c). For the samples with different heating rate, the dehydration starts at the same temperature, but ends at different temperature. This is because the samples with higher heating rate need less time to reach target temperature, and its dehydration time is less. The curves of ln(da /dt) against 1/T of CSH and CH at fixed dehydration degrees range from 0.1 to 0.9 were plotted and showed in Fig. 4. It was observed that the plots of ln(da /dt) against 1/T of CSH and CH were linear. The trend of ln(da /dt) against 1/T plots of CSH varies with dehydration degree (Fig. 4a). In the contrast, all ln(da /dt) against 1/T plots of CH at different dehydration degrees overlap together (Fig. 4b). By making trend lines of the ln(da /dt) against 1/T plots in Fig. 4, the Ea and lnA are determined and showed in Fig. 5. It is showed that the Ea and the lnA of CSH develop with a obviously. And the the Ea and the lnA of CH almost keep the same during the dehydration process. The average Ea of dehydration of CH is 151.82 kJ/mol.
Portlandite Alite Blite Quartz Brownmillerite
Q. Zhang, G. Ye 100 98 96 94 92 90 88 86 84 0
1 K/min 2 K/min
Fig. 3 TG curves of cement paste, CSH and CH
5 K/min 10 K/min 30 K/min
5 K/min 10 K/min
(a) Cement paste 100.0 99.5 99.0 98.5 98.0 97.5 97.0 96.5 96.0
Temperature/°C (b) CSH
1 K/min 2 K/min 5 K/min 10 K/min 30 K/min
Temperature/°C (c) CH
1/T/°C–1 0.0013 0.0018
α =0.5 α =0.6
0 0 0.1 0.2 0.3 0.4 0.5 0.6 0.7 0.8 0.9
(a) CSH Discussion on variation of Ea with progress of reaction The activation energy Ea is the average excess energy that a water molecule must possess to release . A variation of Ea with reaction process implies that systematic change
α =0.1 α =0.2
α =0.4 α =0.5
α =0.7 α =0.8
α =0.8 α =0.9
0.001 0.002 0.003
Fig. 5 Activation energy and lnA determined by isoconversional method
180 25 160 20 140 120 15 100 80 10 60 Ea 40 InA 5 20 0 0 0.1 0.2 0.3 0.4 0.5 0.6 0.7 0.8 0.9
Fig. 4 Plots of ln(da /dt) against 1/T of CSH and CH
of reactivity takes place during the progress of a reaction. The possible reasons of a variation of Ea were discussed by Galwey . The variation of Ea of CH with a is very small (relative standard deviation = 3.85%). This can be explained that
Dehydration kinetics of Portland cement
Verification In order to verify the measured kinetics parameters, the above kinetics model is compared with further experimental data. The above kinetics parameters are computed from the data under different heating rate. But in principle, they are intrinsic parameters, which are applicable for the case under any temperature profile. If an arbitrary temperature–time relation is given, the total mass loss of cement paste at any time can be calculated. The dehydration degrees of CSH and CH can be calculated by numerical method first. The numerical forms of dehydration degree of CH and CSH are showed as following:
aiþ1;CSH ¼ai;CSH þð1ai;CSH Þn A0;i;CSH expðEa;i;CSH =RTi ÞDt ð8Þ aiþ1;CH ¼ ai;CH þ ð1 ai;CH Þn A0;CH expðEa;CH =RTi ÞDt ð9Þ where t is time, i is the time step, Dt is the time step length. Combining the dehydration of CSH and CH, the mass loss in the total dehydration process of cement paste can be characterized as following: Wcem ¼ WCSH aCSH þ WCH aCH
where Wcem is the total mass loss of cement paste, WCSH is the maximum mass loss caused by dehydration of CSH, WCH is the maximum mass loss caused by dehydration of CH. To validate both the kinetics of isothermal and nonisothermal process, the cement paste was heated under a multi-segment temperature program. The sample was heated with rate 5°C/min first. When temperature reached 200°C, the temperature programmer was switched from dynamic heating mode to the isothermal condition for 60 min. At the end of the 60 min, the temperature programmer was switched again to dynamic heating until 400°C. Then the sample was kept in 400°C for another 60 min. At the end of the isothermal process, the sample was heated again with heating rate 15°C/min until 1,000°C. Figure 7 illustrated that the simulated results agreed with the experimental data very well not only in non-isothermal segments but also in isothermal segments. When the heating method was switched from dynamics heating mode to the isothermal condition, the equilibrium state of CSH was not reached immediately. Therefore, the dehydration reaction proceeded at both isothermal segments and nonisothermal segments. Because the activation energy increased along with extent of dehydration, the reaction rate decreased gradually in the isothermal segment.
CSH layer Gel pore
Monolayer of water
CSH globule (5 nm)
the dehydration of CH is a single step reaction. During the reaction process, the energy barrier to bond redistribution of CH almost keep the same. The small variation of Ea might be caused by computational error. The large variation of Ea of CSH with a can be explained by that the dehydration of CSH is a multistep reaction. The CSH gel in hydrated cement paste has consists of many small globules with a disordered layered structure . There are some water molecules absorbed in the interlayer space and surrounding globule (Fig. 6). Because of the complexity of gel structure, different water molecules requires different energy to be released. At high temperature, the monolayer water molecules that surrounds globule are released first, when the interlayer water molecules keep the same. When temperature is sufficiently high, the interlayer water molecules are released finally. Moreover, the CSH structure varies with temperature rising. As Taylor  pointed out, the interlayer spacing shrunk with release of water molecule. The smaller the spacing between CSH layer is, the more energy could be required to dehydrate.
100 120 140 160 180
Fig. 6 A schematic of globulous structure of CSH gel
Fig. 7 Comparison of mass loss measured by thermogravimetry and mass loss curve predicted by kinetics model under complex temperature program
Q. Zhang, G. Ye
In order to characterize the kinetics of the dehydration of different phase in cement paste, a global kinetics of cement paste was considered as the combination of kinetics of CSH and CH. The phases in cement paste was identified by powder XRD. Isoconversional methods [8, 10] were performed to study the dehydration kinetics of CSH and CH. The Ea and the lnA of the dehydration of CSH and CH were determined, respectively. The following conclusions can be drawn: – In the fresh Portland cement paste that has been oven dried at 105°C, CSH and CH are the main hydration products. The minor crystalline phase (like CaCO3) can be neglected during the dehydration. – The Ea of the dehydration of CH is about 151.82 kJ/ mol. The variation of Ea of the dehydration of CH is very small. – The Ea of the dehydration of CSH varies from 83.69 to 371.93 kJ/mol. The variation of Ea of the dehydration of CSH is explained by its complex globulous structure at high temperature. – The global kinetics model of cement paste and its measured parameters were verified by comparing the simulated mass loss with experimental data.
1. Khoury GA, Majorana CE, Pesavento F, Schrefler BA. Modelling of heated concrete. Mag Concr Res. 2002;54(2):77–101. 2. Shaw S, Henderson CMB, Komanschek BU. Dehydration/ recrystallization mechanisms, energetics, and kinetics of hydrated calcium silicate minerals: an in situ TGA/DSC and synchrotron radiation SAXS/WAXS study. Chem Geol. 2000;167(1–2): 141–159. 3. Alonso C, Fernandez L. Dehydration and rehydration processes of cement paste exposed to high temperature environments. J Mater Sci. 2004;39(9):3015–3024. 4. Alarcon-Ruiz L, Platret G, Massieu E, Ehrlacher A. The use of thermal analysis in assessing the effect of temperature on a cement paste. Cem Concr Res. 2005;35(3):609–613. 5. Bazant ZP, Kaplan MF. Concrete at high temperatures: material properties and mathematical models. London: Longman; 1996. 6. Taylor HFW. The water content of calcium sillicate hydrate(I); 1953. 7. Taylor HFW. The dehydration of tobermorite. In: clays and clay minerals, 6th Nat. Conf. Pergamon Press: New York; 1959. p. 101–109. 8. Vyazovkin S, Sbirrazzuoli N. Isoconversional kinetic analysis of thermally stimulated processes in polymers. Macromol Rapid Commun. 2006;27(18):1515–1532. 9. Friedman HL. Kinetics of thermal degradation of char-forming plastics from thermogravimetry: application to a phenolic plastic. J Polym Sci Part C Polym Symp. 1964;6(1):183–195. 10. Brown ME, Maciejewski M, Vyazovkin S, Nomen R, Sempere J, Burnham A, et al. Computational aspects of kinetic analysis: part A: the ICTAC kinetics project-data, methods and results. Therm Acta. 2000;355(1-2):125-143. 11. Galwey AK, LinkBrown ME. Thermal decomposition of ionic solids. Elsevier: Amsterdam; 1999. 12. Galwey AK. What is meant by the term variable activation energy when applied in the kinetic analyses of solid state decompositions (crystolysis reactions)? Therm Acta. 2003;397 (1–2):249–268. 13. Jennings HM. Refinements to colloid model of C–S–H in cement: CM-II. Cem Concr Res. 2008;38(3):275–289.
Acknowledgements The authors thank the Dutch National Science Foundation (STW) for financially supporting the research project on ‘‘Explosive spalling of concrete: towards a model for fire resistant design of concrete elements’’ (code no. 07045). Open Access This article is distributed under the terms of the Creative Commons Attribution License which permits any use, distribution, and reproduction in any medium, provided the original author(s) and the source are credited.